- 66 Views
- Uploaded on
- Presentation posted in: General

Interface-induced lateral anisotropy of semiconductor heterostructures

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Ioffe Physico-Technical Institute, St. Petersburg, Russia

Interface-induced lateral anisotropy of semiconductor heterostructures

M.O. Nestoklon,

JASS 2004

- Introduction
- Zincblende semiconductors
- Interface-induced effects
- Lateral optical anisotropy: Experimental
- Tight-binding method
- Basics
- Optical properties in the tight-binding method

- Results of calculations
- Conclusion

(001)

Plin

The light, emitted in the (001) growth

direction was found to be linearly polarized

This can not be explained by using the Td symmetry of

bulk compositional semiconductor

Td symmetry determines bulk semiconductor bandstructure

However, we are interested in heterostructure properties.

An (001)-interface has the lower symmetry

C’

A’

C

A

The point symmetry of a single (001)-grown

interface is C2v

Electrons and holes with the effective mass

The Kane model takes into account complex band structure of the valence band

and the wave function becomes a multi-component column.

The Hamiltonian is rather complicated…

If we have the rotational axis C∞, we can define the angular momentum component

l as a quantum number

l = 0, ±1, ±2, ±3, …

l = ±1/2, ±3/2, …

Cn has n spinor representations

The angular momentum can unambiguously be defined only for

l = 0, ±1, ±2, ±3, …

l = ±1/2, ±3/2, …

-n/2 <l≤ n/2

C2v contains the second-order rotational axis C2 and does not

distinguish spins differing by 2

For the C2v symmetry, states with the spin +1/2 and -3/2 are coupled in the Hamiltonian.

As a result of the translational symmetry, the state of an electron in a crystal is

characterized by the value of the wave vector k and, in accordance with the Bloch

theorem,

Let us remind that k is defined in the first Brillouin zone. We can add any vector

from reciprocal lattice.

In the absence of translational symmetry the classification by k has no sense.

-X coupling occurs due to translational symmetry breakdown

Schematic representation of the band

structure of the p-i-n GaAs/AlAs/GaAs

tunnel diode. The conduction-band minima

at the and X points of the Brillouin zone

are shown by the full and dashed lines, respectively. The X point potential forms

a quantum well within the AlAs barrier,

with the -X transfer process then taking

place between the -symmetry 2D emitter states and quasi-localized X states within the AlAs barrier.

J. J. Finley et al, Phys. Rev. B, 58, 10 619, (1998)

E.L. Ivchenko, A. Yu. Kaminski, U. Roessler,

Phys. Rev. B 54, 5852, (1996)

Type I

Type II

The main difference is that interband optical transition takes place only at the interface

in type-II heterostructure when, in type-I case, it occurs within the whole CA layer

(001)

Plin

type I

type II

A.V. Platonov, V. P. Kochereshko,

E. L. Ivchenko et al., Phys. Rev. Lett. 83, 3546 (1999)

Situation is typical for type-II

heterostructures.

Here the anisotropy is ~ 60%

F. Fuchs, J. Schmitz and N. Herres,

Proc. the 23rd Internat. Conf. on Physics of Semiconductors,

vol.3,1803 (Berlin, 1996)

C

A

C

A

C

A

…

…

…

…

V

?

?

In

As

?

As

In

As

In

In

As

?

?

Al

Sb

Al

?

GaAs

(strained)

GaSb

GaSb

A.A. Toropov, O.G. Lyublinskaya, B.Ya. Meltser,

V.A. Solov’ev,A.A. Sitnikova, M.O. Nestoklon, O.V. Rykhova, S.V. Ivanov, K. Thonke and R. Sauer,

Phys. Rev B, submitted (2004)

E.L. Ivchenko and M.O. Nestoklon, JETP 94, 644 (2002);

arXiv http://arxiv.org/abs/cond-mat/0403297 (submitted to Phys. Rev. B)

- A tight-binding approach has been developed in order to calculate the electronic and optical properties of type-II heterostructures.
- the theory allows a giant in-plane linear polarization for the photoluminescence of type-II (001)-grown multi-layered structures, such as InAs/AlSb and ZnSe/BeTe.

If crystal lattice has the symmetry transformations

Then the Hamiltonian is invariant under these transformations:

where is point group representation

- Для описания экспериментальных данных необходим
- учёт спин-орбитального расщепления валентной зоны
- для описания непрямозонных полупроводников “верхние орбитали” (s*)

~ 20-зонная модель. 15 параметров